Photoacoustic effects in nanocomposite structure ‘porous silicon-liquid’
- First Online:
- Cite this article as:
- Andrusenko, D., Isaiev, M., Kuzmich, A. et al. Nanoscale Res Lett (2012) 7: 411. doi:10.1186/1556-276X-7-411
- 2.1k Downloads
Photoacoustic effect in nanocomposite structure ‘porous silicon-liquid’ has been investigated. Main mechanisms involved in the formation of photoacoustic signal in such structures have been experimentally studied. Liquids with different viscosity (ethanol and acetone) filling the nanopores have been used. A proposed mathematical model describing the photoacoustic signal formation was found to be in good agreement with the experimental results. The role of thermally induced pressures provoked by the liquids confined inside the nanopores in the photoacoustic process has been analyzed.
KeywordsPorous silicon Photoacoustic and photothermal phenomena Nanocomposite structures
‘Porous matrix-liquid’ structures are widely used in such fields of science and technology as medicine, biology, geology, chemistry, etc.. This is important to know mechanical, thermal, optical, and other properties of these structures from an application point of view. Investigations of such properties allow to obtain a lot of useful information about the hosting porous matrix, behavior of the liquids in the confining pore spaces, (for instance, properties of nanofluids), as well as about the whole composite porous matrix-liquid structure.
Photoacoustic (PA) techniques have proven to be capable for studying of porous materials and layered structures. This is mainly due to the fact that, in most cases of their practical implementations, they are nondestructive. In particular, it has been already demonstrated the possibility of using PA techniques for the study of fluid migration in porous materials. Moreover, the PA signal detected by a piezoelectric registration was shown to be sensitive both to thermally induced pressures (TIP) of the liquids localized inside the pores of the composite ‘porous silicon-liquid’ system and to the pressure relaxation phenomena. Thus, understanding of the PA transformation effects in the porous materials with empty or filled pores enables development of new experimental and diagnostic methods (including in situ methods in the manufacturing process) for characterization of such materials and composites.
In this paper, photoacoustic signals recorded with a piezoelectric transducer in the nanocomposite structure porous silicon-liquid are theoretically simulated and experimentally measured. In particular, the influence of thermally induced pressures of the liquid in the pores on shape and parameters of the photoacoustic response is analyzed in detail.
The mesoporous silicon layers were prepared by anodic etching. Highly boron-doped p+-type (0.01 to 0.02 Ω.cm) double-sided polished (100)-oriented Si wafers were electrochemically treated. Etching solution contained a 1:1 volume mixture of concentrated aqueous HF acid (49%) and pure ethanol. A constant anodic current density depending on the desirable porosity value was applied for various times to ensure different thicknesses of the final porous layer. A permanent stirring of the etching solution was applied in order to evacate hydrogen bubbles formed during the anodization process.
where c and ρ are the heat capacity and volume density, respectively; χ, the thermal conductivity. The boundary conditions for this equation are as follows:
where ωn =2πn/Tp (n is the integer number); n = 0 in the sum term corresponding to the averaged intensity distribution for one period has been omitted.
The constants,,, and can be obtained from the boundary conditions.
Thermally induced pressure
where ε is the porosity, βTl is the coefficient of volume thermal expansion of the liquid, K is the fluid permeability of the porous silicon, η is the liquid’s viscosity, β is the liquid’s compressibility.
The constants and can be obtained from the boundary conditions.
Photoacoustic signal formation
This source consists of two components: (1) the thermoelastic stresses of the porous matrix and monocrystalline Si wafer (first term) as well as (2) the TIPs of the liquid inside the pores (second term).
whereis the function describing the voltage excitation performance depending on a point at which the elastic force is applied.
Results and discussion
As one can see from Figures2 and3, the PA signal obtained for the porous Si-liquid structure is significantly different from the PA signal obtained on the similar structure without liquid (see reference, for example). In particular, at least two main characteristic features of the transient PA signals recorded from the nanocomposite structure porous Si-liquid can be noted: (1) a sharp initial rise is followed by (2) a more or less pronounced bend. These features become to be well resolved especially for relatively high porosity and larger thickness values, and the following characteristic sequence can be observed: sharp rise -maximum -bend -minimum -additional slight signal growth. These features are ensured by the TIP appearance (first feature) and relaxation (second feature) of the liquid inside the pores. The TIP arises due to significant differences between the parameters of the liquid and solid matrices (in particular, thermal expansion coefficients and compressibility). The time positions of these features depend on the thermophysical properties of liquid and solid matrix composites, fluid viscosity, the permeability K, and the thickness of the porous layer.
As we can see in Figure3a, the first feature shifts toward the lower time range when thermal conductivity increases. It can be explained by the fact that thermal energy achieves more rapidly in Si wafer. Consequently, it leads to (a) the decrease of the liquid heating and (b) the general changes of relation between thermoelastic stresses and TIP contributions in the resulting structural deformations. Figure3b illustrates influence of porous matrix permeability on the temporal shape of the PA signal. The first feature is shifted to the lower time edge with increasing permeability. The similar qualitative result is observed if the liquid viscosity decreases. This is due to the fact that the TIP relaxation time increases as a result of decreasing dissipative forces. Taking into account all these effects, the experimental PA signals can be perfectly fitted by the mathematical model described previously and by considering general thermophysical properties of the porous matrix-liquid composite, viscosity, permeability K, and thickness of the porous layer (for example, see comparison between experimental and simulated signals shown in Figure3).
In this paper, experimental and theoretical investigations of photoacoustic effect in nanocomposite porous silicon-liquid structures have been reported. The role of thermal-induced pressures of liquids confined inside the nanopores in formation of the photoacoustic signal has been highlighted. The influence of liquid and porous matrix parameters on the temporal shape of the photoacoustic signal has been demonstrated.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.